Journal of Emerging Trends in Engineering and Applied Sciences (JETEAS) 3(4) 718-724 (ISSN: 2141-7016)
Optimum Mix Design for Minimum Concrete Strength Requirement
Using Akure Pit-sand as Fine Aggregate
S.A. Alabi, L.M. Olanitori, and J.O. Afolayan
Civil Engineering Department, Federal University of Technology, Akure, P.M.B 704, Nigeria.
Corresponding Author: S.A. Alabi ___________________________________________________________________________ Abstract This paper highlights the properties of pit-sand commonly used as fine aggregate and the resulting concrete produced in Akure, South-west of Nigeria. The research into the characteristics and behaviour of locally available aggregates is expected to improve the knowledge of the structural engineers as well as all the civil engineers that make use of concrete. The main aim of this research is to develop optimum proportioning of local aggregate suitable for the customization of BS8110 (1997) in Nigeria. Linear programming technique has been applied to a concrete mix design having least cost while satisfying given water-cement ratio; the specified limits for the range of acceptable workability, expressed in terms of the compacting factor; absolute volume constraint and the specified compressive strength. The objective function, for which a minimum is sought, is the cost of concrete per cubic meter, expressed as the sum of the unit costs of the individual ingredients. The characteristic strength of the concrete at 28 days was found to be 10.44 N/mm2 at an optimal mix ratio of 1:2:5 and water-cement ratio of 0.77. __________________________________________________________________________________________ Keywords: pit-sand, concrete, compressive strength, optimization. __________________________________________________________________________________________ INTRODUCTION Concrete is presently the most common building material in Nigeria, hence careful consideration must be given to factors that affect its strength. To ensure the overall good performance of a reinforced concrete structure, the quality of its constituent materials must be ensured (Afolayan, 1993). Structural collapse of reinforced concrete buildings is usually an outcome of progressive deterioration of the various components forming the structural unit as a result of improper mix ratio or ignorance in the use of locally available fine aggregate containing impurities, which consequently affect the overall mix (Babatunde and Opawole, 2009). Mix ratio can affect the strength and stability of a reinforced concrete structure just as the size, the shape and the grading of the aggregate will do (Alexander and Mindess, 2008). However, the incidence of material failure of concrete in recent years in Nigeria is a clear indication that the professional engineers in the country may not know enough about their concrete. To some extent, the ignorance may cause negligence in the selection of correct ingredients for mixing, to achieve a suitable mix, and obtain a technically sound execution of concrete works (Ayininuola and Olalusi, 2004). The standard mix of approximately 1:2:4 (ratio of cement to fine and to coarse aggregate) is expected to give a compressive strength of 20 N/mm2 at 28 days (Table 5 of BS8110 1997) could not achieved using aggregates available in Akure metropolis. Olanitori and Olotuah (2005) achieved a concrete of compressive strength between 8 N/mm2 and 12 N/mm2. In the light
of the shortcomings that may be associated with aggregates, it has become imperative to research into these aggregates that are readily available in our environment and know at what optimum mix ratio a minimum concrete strength is obtained. The research into the characteristics and behaviour of locally available aggregates is expected to improve the knowledge of the structural engineers as well as all the civil engineers that make use of concrete for civil engineering works. LOCATION, MATERIALS AND METHODS Location The study area is Akure, the administrative capital of Ondo State. Akure became the state capital of Ondo State in 1976. The town is located within 70 15 north of the Equator and Longitude 50 05 East of the Greenwich Meridian. In 2006, the provisional population for Akure was put at 353,211 (2006 census) out of which 175,494 are male and 177,716 are female. Figure 1.0 shows the location of Akure in Ondo state as well as Nigeria. Generally, the people have almost the same life pattern. A large majority are civil servant and a consistently people of entrepreneurship. The increased relative political influence of Akure as a State capital since 1976, when Ondo State was created has been partly responsible for its rapid development. This is because, the decentralization exercise, which accompanied the policy that led to the creation of the State led to the creation of jobs, which attracted many people.
Journal of Emerging Trends in Engineering and Applied Sciences (JETEAS) 3 (4): 718-724 Scholarlink Research Institute Journals, 2012 (ISSN: 2141-7016) jeteas.scholarlinkresearch.org
Journal of Emerging Trends in Engineering and Applied Sciences (JETEAS) 3(4) 718-724 (ISSN: 2141-7016)
Figure 1.0: Map of Ondo state Showing Study Area (Source: Rectas Archive, Ile Ife, Nigeria) MATERIALS Sand Akure pit-sand is an aggregate whose grain sizes range from 0.075 mm to 2.36 mm. Chemical analysis showed that the material contains various minerals like SiO2, Al2O3, Fe2O3, CaO, MgO, Na2O, K2O and TiO, which provide specifically a diversity of physical and mechanical properties. In spite of the reactivity of some minerals with cement, sand is considered as an inert component that may affect the resulted mix property by its texture, size, distribution, strength and other secondary properties. In general, sand contains water, some of which is absorbed within and some other is attached to the surface. The latter is a cause of variation of mix properties because of its downward movement which makes the water content non-uniform. Table 1 displays the properties of pit- sand sample from Akure, Nigeria.
Table 1: Determined properties of Pit-sand from Akure Property Value
Specific gravity, Gs 2.34
Bulk Density (kg/m3) 1390
Fineness modulus 1.82
Cement Cement is a hydraulic powder that reacts with water and hardens under water to form a hardened rock. In this research ordinary Portland cement is used. In concrete, cement is the first component that reacts with water; its reaction is always accompanied with hydration heat whose value may be high or low according to the cement components mainly including: C2S, C3S, C3A, C4AF and gypsum. Strength of cement is of first importance because its role is to bond all aggregates together to form a unique rock.
Coarse Aggregate The type and source of coarse aggregate used in the production of concrete in Akure, Metropolis has a considerable influence on the compressive strength of concrete. Crushed but smooth coarse aggregate of the maximum size of 14 mm is commonly used in making concrete. The properties of the coarse aggregate used in this investigation are as listed in Table 2. Table 2: Coarse aggregate properties
Properties Value Fineness modulus 5.78 Specific gravity, Gs 2.65 Bulk Density (kg/m3) 1635 Absorption 1.86
METHODS Proportioning of concrete ingredient using linear programming technique was focused. Linear equations were solved using the Microsoft Excel Spreadsheet Solver and preliminary concrete mix ratio of 1:2.1:1.8 was obtained. This primary concrete mix ratio was used to generate a set of other trial concrete mix ratios, i.e., 1:2:4.5; 1:2:5; 1:2.5:6; and 1:3:5. The soil (pit-sand) sample used as fine aggregate in concrete was oven-dried for 24 hours before further tests were carried out. The sand and granite used as aggregates were graded using the sieve sizes for grading according to BS812: part 103 (1985). Hence, the percentage passing through each set of sieves was determined. The concrete ingredients were then mixed using the method of batching by weight in accordance with the provision of BS 812: Part 104 (1985). Pit-sand having maximum particle size of 2.36 mm, determined from particle size distribution method, was first measured, and spread with shovel, after which ordinary Portland cement was added and thoroughly mixed. The resulting mix was then mixed with coarse aggregate (granite) of maximum particle size of 14 mm and the required amount of water. The resulting concrete was poured in the standard concrete cube mould of 150 x 150 x 150 mm in three layers. Each layer was given 25 blows for compaction using British Standard rod as recommended by BS1881: Part 111 (1983). The fresh concrete was tested in accordance with British Standards (1881: Part 102 (1983), BS812: part 103 (1985), BS1881: Part 106 (1983)) for slump, compacting factor, and Air-entrained volume. The concrete cubes were removed after 24 hours from the moulds, weighed and kept under water for curing in the curing tank. After every 7 days 3 samples of concrete cube were removed from the curing tank, weighed and tested for compressive strength. The values of compressive strength were read and recorded. The same procedure was followed for the trial concrete mix ratios 1:2:4; 1:2:4.5; 1:2:5; 1:2.5:6; and 1:3:5. RESULTS AND DISCUSSION Results of tested properties of materials The properties of the fine and coarse aggregates from Akure are as presented in Table 3. It is clear from the
Journal of Emerging Trends in Engineering and Applied Sciences (JETEAS) 3(4) 718-724 (ISSN: 2141-7016)
results that both materials exhibit qualities lower than the recommended minimum in BS812: Part101 (1985).
Table 3: Summary of materials properties in the Study
Pit-sand Coarse Cement
Fineness Modulus 1.82 5.78 - Specific gravity, Gs 2.34 2.65 3.13 Bulk Density (kg/m3) 1390 1635 1497 Absorption 2.42 1.86 -
Particle Size Distribution of Akure Pit-Sand According to the Unified Soil Classification System, the sand sample is a fine grained soil (sand) because more than half of the coarse fraction is between the No 4 (4.75 mm) and No 200 (0.075 mm) sieve size. However, from Figure 2, the coefficient of uniformity, Cu and coefficient of curvature (Cz) are 2.59 and 1.06 respectively. Since, Cu < 4 and Cz = 1.06 which is between 1 and 3 in the Unified Soil Classification System, the soil is classified as poorly graded sand. More than half of the coarse fraction is not retained on the No 4 sieve showing that the aggregate is poorly distributed. From Figure 2, the grading of coarse aggregate does not comply with the requirement of BS812: Part101 (1985) which has effect on the water requirement of a concrete mix.
Figure 2: Particle size distribution curve for Akure pit-sand
Figure 3: Particle size distribution curve for granite
Chemical Composition of Pit-sand Figure 4 gives the result of chemical composition analysis carried-out on the pit-sand used as fine aggregate. The Akure pit-sand contains higher percentage of undissolved metal and lower silicate (77.40%) as compared with some standard sand like Ottawa sand (silicate of about 99.3%) in Canada which affect the bond between the matrix and the aggregate particles and thus the strength of concrete (Fijabi, 2011).
Figure 4: Percentage metal oxide present in Akure pit-sand Application of Linear Programming to Concrete Ingredient Proportioning The concept of linear programming technique has been applied to concrete mix design having least cost while satisfying given workability requirements, minimum water-cement ratio and the specified compressive strength in the hardened state. The objective function, for which a minimum is sought, is the cost of concrete per cubic meter, expressed as the sum of the unit costs of the individual ingredients.
Particle size in mm
Required Concrete Strength Constraint Compressive strength of concrete has been generally taken to be a function of the water-cement ratio which is given as
( )cuf M A D (1) In equation (1), (water-cement ratio by weight); and fcu, M and D are compressive strength in N/mm2 at 28 days, slope of a straight line (obtained from strength versus water-cement ratio relationship) and 2 2cuD f M A Where and are maximum compressive strength and water-cement ratio on the strength versus water-cement ratio relationship The strength constraint then assumes the form W 0.77*C 0 (2) where W = quantity of water in kg per unit volume of concrete; C = quantity of cement in kg per unit volume of concrete. Equation (2) is meant to provide adequate concrete strength (Cannon and Krishna Murti, 1971) Workability Constraint The following relationship for workability, suggested by Murdock, (1960) has been utilized in this present study.
in which CF = compaction factor; FS = surface index of the aggregate; FA = angularity index of the aggregate; and Av = aggregate-cement ratio by volume. To express Av in terms of the aggregate-cement ratio by weight; we have
(4) where GC = specific gravity of cement, GA = specific gravity of aggregate, A/C = aggregate-cement ratio by weight. To ensure adequate workability, a lower limit of compacting factor was imposed. Substituting Equation (4) into Equation (3) and solving mathematically we have 7.40W B2*C B3*CA B4*FA 0 (5) Where
3 0.4958FA FAFA
GCB FS FA CFLGA
4 0.4958CA CACA
GCB FS FA CFLGA
in which CFL = lower limit of compacting factor, FS = surface index of the aggregate, FA = angularity index of the aggregate, C = cement, W = Water. The parameters FAFA, FSFA, FACA, FSCA, GC, GACA, GAFA, and CF are taken to be 2, 0.356, 2, 1.075, 3.13, 2.65, 2.34, and 0.850 respectively. Hence, substituting all the
parameters into Equation (6); (7); and (8), the limiting workability constraints assume the form: 7.40*W 1.20*C 1.15*CA 0.39*FA 0 (9) Water to Cement Ratio Constraint Table 6.3.4 of ACI, (1991) gives the maximum permissible water-cement ratio for concrete in severe exposure. This specification results in a constraint expressed as: W/C R or W 0.5*C 0 (10) assuming R = 0.5 Volume Constraint Equation (11) constrains the total volume of water, cement, coarse aggregate, fine aggregate to the concrete volume, V
w c ca fa
W C CA FA VG G G
Where GC = specific gravity of cement = 3.13, Gca = specific gravity of coarse aggregate = 2.65, Gfa = specific gravity of fine aggregate = 2.34, = density of water which is taken to be 1000 kg/m3. Substituting these data into Equation (11) we have 0.001W + 0.32C + 0.37CA+ 0.38FA= 2604.16 (12) Objective Function and Constraints The objective function, for which a minimum is sought, is the cost of concrete per cubic meter, expressed as the sum of the unit costs of the individual ingredients. That is, Min Z = 33C + 0.5FA + 3.5CA + 0.05W (13) Where C, FA, CA and W are cement, fine aggregate, coarse aggregate and water respectively.The objective function is subject to the constraints expressed in Equations (2), (9), (10) and (12). The Result of Optimization The optimisation was performed using the Microsoft Excel Spreadsheet. The optimum mix ratio obtained was 1:2.1:1.8 for C: FA: CA Characteristic Compressive Strength The characteristic compressive strength, fcu for the concrete at different ages was obtained from
1.64cu mf f (14) Where fcu is the characteristic compressive strength of the concrete at any age, fm is the mean target strength of the concrete at any age and is the standard deviation of the sample values. From Figure 4 the results clearly show that the materials used were of poor quality resulting in low characteristic strength at 28 days as compared with the recommendation given by BS8110: Part 1 (1997).
Figure 5: Characteristic compressive strength, fcu of concrete for varying mixes Fresh Concrete Properties From Table 4, the compactor factors obtained for all concrete mix ratios show that concrete is neither too fluid nor too solid. The consistency of the concrete measured by slump values, the void volume, vebe-time and the density of the concrete for the tested concrete mix ratios using Akure pit-sand are in compliance with the recommendation given by BS812: Part101 (1985). Table 4: Fresh concrete properties
Effect of Concrete Water Absorption on Characteristic Strength of Concrete at Different Ages Figures 6 to 11 display the relationship between compressive strength and the percentage of water absorption for different concrete mix ratios. The pit-sand used has the ability to retain higher moisture content, which made it react with alkalis from the cement to cause cracking which in turn reduced the compressive strength of concrete. The maximum sizes of aggregates used in this research are smaller compared with the maximum size of aggregate given in BS812: Part 106 (1985). This implies that the smaller the maximum size of aggregate, the higher the water content, the higher the slump value and the lower the compressive strength of concrete. Generally, there is no regular pattern for describing the variation of concrete strength with water absorption for the type of
aggregates used in this study. This observation supports the fact that the resulting compressive strength should be treated probabilistically.
Figure 6: Compressive strength against % water absorption for mix ratio 1:2.1:1.8
Figure 7: Compressive strength against % water absorption for mix ratio 1:2:4
Mix Ratio Fresh Concrete Properties
Compaction Factor Slump
Air Content (%)
Concrete Density kg/m3
1:2.8:1.8 0.99 52 2.5 2379.26 1.44 1:2:4 0.94 56 2.2 2515.56 2.31
1:2:4.5 0.93 63 2.6 2512.59 2.66 1:2:5 0.94 65 2.4 2509.63 2.53
1:2.5:6 0.96 54 2.3 2462.22 2.02 1:3:5 0.95 58 2.5 2456.30 2.25
Figure 8: Compressive strength against % water absorption for mix ratio 1:2:4.5
Figure 9: Compressive strength against % water absorption for mix ratio 1:2:5
Figure 10: Compressive strength against % water absorption for mix ratio 1:2.5:6
Figure 11: Compressive strength against % water absorption for mix ratio ratio 1:3:5 CONCLUSION Physical and chemical properties of commonly used aggregates in one of the cities in the south-western Nigeria were investigated. The concept of optimization was applied to concrete mix design having least cost while satisfying the given concrete workability requirements and the specified compressive strength in the hardened state. The design variables in the optimization process are cement, aggregates (fine and coarse), and water. Compressive strength which is the function of the water-cement ratio was used to establish the required strength constraint from assumed cylinder strength versus water-cement ratio relationship. The optimization process was done using the Microsoft Excel Spreadsheet Solver of linear programming. Consequently, the optimum mix ratio of 1:2.1:1.8 for was obtained. This mix was tested along with other experimental trials. Based on experimental tests the optimum coarse aggregate/total aggregate and total aggregate/cement ratios were found to be 0.46 and 3.9 respectively at an optimal mix of 1:2:5. The concrete compressive strength at 28 days using a mix of 1:2:4 for the local available materials was found to be 10.13 N/mm2 as compared with the minimum compressive strength of 20 N/mm2 recommended by BS8110: Part1 (1997). The experimental value is therefore 50% of the minimum strength recommended. However, the compressive strength at 28 days corresponding to the experimental optimal was 10.44 N/mm2 with water-cement ratio of 0.77. REFERENCES ACI, 1991. Standard Recommended Practice for Selecting Proportions for Normal Weight Concrete. Farmington Hill, Michigan: American Concrete Institute, New York, NY, A.C.I. Standard 211.1-91.
Afolayan, J.O, 1993. Structural Synthesis and Quality Control. Proceedings of the 1st African-USA International Conference on Manufacturing Technology, 11-14, pp 447-457. Alexander, M.G. and Mindess, S, 2008. Aggregates in Concrete.http://www.toolbase.org/Technology-Inventory/Foundations/concrete-aggregate-substitutes#top, Ayininuola, G.M. and Olalusi, O.O, 2004. Assessment of building collapsed in Nigeria, Lagos and Ibadan case study. Department of Civil Engineering, University of Ibadan.African Journal of Science and Technology (AJST), Science and Engineering Series, Vol 5, No 1, pp73-78 Babatunde, S.O and Opawole, 2009. Assessment of failure of Building components in Nigeria. Journal of Building Appraisal 4, pp 279-286. British Standard Institution 8110, 1997. Structural Use of Concrete Part 1: Code of practice for design and construction. Sector Board for Building and Civil Engineering, published under the authority of the Standards Board, London, London. British Standard Institution 5328, 1983. Testing concrete: Methods for determination the Compressive strength of concrete. Published under the authority of the Board of BSI, the direction of the Cement, Gypsum, Aggregates and Quarry Products Standards Committee. London. British Standard Institution 812, 1985. Testing aggregates, Part 103: Methods for determination of particle size distribution Section 103.1 Sieve tests. Published under the authority of the Board of BSI, the direction of the Cement, Gypsum, Aggregates and Quarry Products Standards Committee, London. British Standard Institution 812, 1985. Testing aggregates, Part 104: Methods for determination of particle size distribution Section 103.1 Sieve tests. Published under the authority of the Board of BSI, the direction of the Cement, Gypsum, Aggregates and Quarry Products Standards Committee, London. British Standard Institution 1881, 1983. Testing concrete, Part 111: Method for making test cubes from fresh concrete. Published under the authority of the Board of BSI, the direction of the Cement, Gypsum, Aggregates and Quarry Products Standards Committee, London. British Standard Institution 1881, 1983. Testing concrete, Part 102: Method for determination of Slump. Published under the authority of the Board of BSI, the direction of the Cement, Gypsum, Aggregates and Quarry Products Standards Committee, London.
British Standard Institution 1881, 1983. Testing concrete, Part 106: Methods for determination of air content of fresh concrete. Published under the authority of the Board of BSI, the direction of the Cement, Gypsum, Aggregates and Quarry Products Standards Committee, London. British Standard Institution 812, 1990. Testing aggregates Part 101: Guide to sampling and testing aggregates. Published under the authority of the Board of BSI, the direction of the Cement, Gypsum, Aggregates and Quarry Products Standards Committee, London. Cannon J.P. and Krishna Murti, G.R, 1971. Concrete Optimized Mix Proportioning (Comp). Pergamon Press, Inc Printed in the United States. Cement and concrete research,, Vol. I, pp. 353-366. Fijabi, O.P, 2011. Geotechnical Properties of Some Selected Soils in Nigeria. Final Thesis Seminar, Civil Engineering Department, the Federal University of Technology, Akure, Nigeria. Unpublised. Murdock, L. J, 1960. The Workability of Concrete. Magazine of Concrete Research, Vol. 12, No. 36, pp. 135-144. Olanitori L.M. and Olotuah A.O, 2005. The effect of clayey impurities in sand on the crushing strength of concrete (a case study of sand in Akure metropolis, Ondo State, Nigeria). Proceedings of 30th Conference on Our World in Concrete and Structures, Singapore, 23-24, pp 373-376.
Click here to load reader